Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.


 Lucas Short
 1 years ago
 Views:
Transcription
1 49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates. C. B. York * University of Glasgow, Glasgow, Scotland, G12 8QQ Stacking sequence listings are presented for fully uncoupled Extensionally Isotropic (EILs), Fully Isotropic (FILs) and QuasiHomogeneous Orthotropic (QHOLs) angleply Laminates, with up to 21 plies. All are subsets of a definitive list of Fully Orthotropic Laminates (FOLs), containing generally nonsymmetric stacking sequences that are characterized in terms of angle and crossply subsequence symmetries. Dimensionless parameters are given for each stacking sequence, from which the ABD matrix is readily derived. Expressions relating these dimensionless parameters to the wellknown lamination parameters are also given, together with graphical representations of the feasible domains for π/3 and π/4 EILs and angleply QHOLs containing two and three ply orientations. The feasible domain for π/3 FILs is represented graphically by a single point, whereas the domain for angleply QHOLs containing four ply orientations is represented by a single stacking sequence. Nomenclature A,A ij = extensional (membrane) stiffness matrix and its elements (i,j = 1, 2, 6) B,B ij = bendingextensioncoupling stiffness matrix and its elements (i,j = 1, 2, 6) D,D ij = bending (flexural) stiffness matrix and its elements (i,j = 1, 2, 6) H = laminate thickness (= n t) n = number of plies in laminate stacking sequence N x,n y = inplane axial load per unit length. N xy = inplane shear flow. M x,m y = bending moments per unit length about principal axes. M xy = twist moment per unit length. Q ij = reduced stiffness (i,j = 1, 2, 6) Q ij = transformed reduced stiffness (i,j = 1, 2, 6) t = ply thickness x,y,z = principal axes ε x,ε y = inplane axial strains. γ xy = inplane shear strain. κ x,κ y = curvatures about principal axes. κ xy = twist curvature. ξ 1,ξ 2 = lamination parameters for extensional stiffness (ξ 1 = ξ A 1,ξ 2 = ξ A 2 ) ξ 9,ξ 10 = lamination parameters for bending stiffness (ξ 9 = ξ D 1, ξ 10 = ξ D 2 ) ζ,ζ ±,ζ,ζ = bending stiffness parameter for laminate, and angleply and crossply subsequences +,,± = angle plies, used in stacking sequence definition, = crossplies, used in stacking sequence definition Matrix subscripts 0 = All elements zero F = All elements finite I = Isotropic form, see Eqs. (5) (7) S = Specially orthotropic form, see Eqs. (3)  (4) * Senior Lecturer, Department of Aerospace Engineering, James Watt Building. 1 Copyright 2008 by C. B. York. Published by the, Inc., with permission.
2 Keywords Stacking Sequences; Fully Uncoupled Laminates; Extensionally (or Membrane or Quasi) Isotropic Laminates; Fully Isotropic Laminates; Bending Stiffness Parameters; Lamination Parameters; Feasible Domains. I. Introduction omposite laminate materials are typically characterized in terms of their response to mechanical (and/or thermal) loading, which is generally associated with a description of the coupling behavior, unique to this type C of material, i.e. coupling between inplane (i.e. extension or membrane) and outofplane (i.e. bending or flexure) responses when B ij 0 in Eq. (1), coupling between inplane shear and extension when A 16 = A 26 0, and coupling between outofplane bending and twisting when D 16 = D N N N x y xy A11 A12 A16 ε x = A22 A26 ε y + Sym. A66 τ xy B11 Sym. B B B B B κ x κ y κ xy M M M x y xy B11 B12 B16 ε x D11 D12 D16 κ x = B22 B26 ε y + D22 D26 κ y (1) Sym. B66 τ xy Sym. D 66 κ xy Whilst Eq. (1) describes the wellknown ABD relation from classical laminate plate theory, it is more often expressed using compact notation: N M A B ε = (2) B D κ The coupling behavior, which is dependent on the form of the elements in each of the extensional (A), coupling (B) and bending (D) stiffness matrices is now described by an extended subscript notation, defined previously by the Engineering Sciences Data Unit, or ESDU 1 and subsequently augmented for the purposes of this article. Hence, balanced and symmetric stacking sequences, which generally possess bending anisotropy, give rise to coupling between outofplane bending and twisting and are referred to by the designation A S B 0 D F, signifying that the elements of the extensional stiffness matrix (A) are specially orthotropic in nature, i.e. uncoupled, since A 16 = A 26 = 0, (3) the bendingextension coupling matrix (B) is null, whilst all elements of the bending stiffness matrix (D) are finite, i.e. D ij 0. Laminates possessing extensional anisotropy give rise to coupling between inplane shear and extension only and, by the same rationale, are referred to by the designation A F B 0 D S, signifying that all elements of the extensional stiffness matrix (A) are finite, i.e. A ij 0, the bendingextension coupling matrix (B) is null, and the elements of the bending stiffness matrix (D) are specially orthotropic in nature, i.e. uncoupled, since D 16 = D 26 = 0 (4) The A F B 0 D S designation is not listed as part of the ten laminate classifications described in the ESDU data item 1, but is however the subject of a recent article 2, identifying the definite list of A F B 0 D S stacking sequences with up to 21 plies, thus complementing a new definitive list 3 of Fully Orthotropic Laminates or FOLs. Note that the term for FOLs is synonymous with specially orthotropic laminates, which possess none of the coupling characteristics described above and are represented by the designation A S B 0 D S. 2
3 This article presents the characterization of uncoupled Extensionally Isotropic Laminates or EILs, with the designation A I B 0 D S and Fully Isotropic Laminates or FILs, with the designation A I B 0 D I. These laminates represent subsets of FOLs and are therefore contained within the definitive list 3, since in addition to the specially orthotropic form of each matrix, see Eq. (3), elements simplify further in EILs and the designation A S is replaced with A I to indicate that: and A 11 = A 22 (5) A 66 = (A 11 A 12 )/2 (6) and further still in FILs, in which the designation D S is replaced with D I to indicate that: D ij = A ij H 2 /12, (7) where H is the laminate thickness, corresponding to the total number of plies, n, of thickness t. QuasiHomogeneous Orthotropic Laminates, or QHOLs, similar to the QuasiHomogeneous Anisotropic Laminates, or QHALs, described and patented by Wu and Avery 5, satisfy Eq. (7) but not Eqs. (5) and/or (6). QHOLs (QHALs) offer matching orthotropy (anisotropy) in both extensional and bending stiffness. Note that QHOLs are developed herein for general ply angle ±θ, but the same stacking sequences produce QHALs when +θ θ. Fully orthotropic laminates, from which all stacking sequences presented in this article are derived, minimize distortion during manufacturing and maximize compression buckling strength 6, particularly in comparison to balanced and symmetric laminates, which are commonly adopted in aircraft and spacecraft construction, despite the fact that such laminates generally possess bending anisotropy. Valot and Vannucci provide recent examples of laminate stacking sequences for FOLs with antisymmetric sequences 7, following a previous article 8 on FILs. These two articles are part of, and provide reference to, a growing number of related articles by a community of coworkers addressing the development of laminate stacking sequences exhibiting a range of physical characteristics, all of which refer back to an original article by Caprino and CrivelliVisconti 9, identifying the specially orthotropic angleply laminate with eight plies. Much of this related work has been focused on laminate stacking sequences for QuasiIsotropic or Extensionally Isotropic Laminates (EILs), Fully Isotropic Laminates (FILs), and laminates with material homogeneity. However, with the exception of FILs, these material characterizations generally provide little or no distinction between laminates with or laminates without coupling behavior. For instance, the quasihomogenous laminate, which is defined as possessing the same elastic propertied in both flexural and membrane actions, but with no coupling between these two actions, may be designated as either A F B 0 D F or A S B 0 D S, and extensionally isotropic laminate may be designated as either A I B 0 D F or A I B 0 D S. Such sequences have been obtained through an inverse polar (or Mohr s circle) representation method developed by Verchery and coworkers, which is acknowledged 10 to be similar to the method presented previously by Tsai and Pagano 11. By contrast, original work by Bartholomew 12,13, which forms the basis of the Engineering Sciences Data Unit (ESDU) publication 14 for the so called definitive list of fully orthotropic angleply laminates with designation A S B 0 D S, precedes the findings of Caprino and CrivelliVisconti 9, but appears to have been completely overlooked in the literature described above. This published list of stacking sequences contains 75 symmetric sequences for laminates with up to 21 plies, 653 antisymmetric sequences for laminates with up to 20 plies and 49 additional nonsymmetric (asymmetric) sequences, which were derived by combining the symmetric and antisymmetric sequences. Further inspection reveals that there are no angleply laminates possessing specially orthotropic properties with fewer than 7 plies. Indeed, there is only one generic 7layer angleply antisymmetric stacking sequence. This number increases to 233 generic antisymmetric sequences with 20 ply layers. There are no symmetric stacking sequences with less than 12 layers, and only 25 combinations with 20 layers. These twentyfive generic stacking sequences possess balanced and symmetric combinations of angle plies, together with cross plies, which may be 0 and/or 90, symmetrically disposed about the laminate midplane; all possess angleply layers on the outer surfaces of the laminate. The term generic is used here to describe the form of the stacking sequences adopted, defined by three parameters: +, and, relating to positive and negative angle plies with general orientation, θ, and cross ply, respectively. The derivation 12,13 adopted in the ESDU data item 14, made the explicit assumption that cross plies, as well as angle plies, are symmetrically disposed about the laminate midplane, i.e. the mixing of 0 and 90 plies is 3
4 permitted only in one half of the laminate, which is then reflected symmetrically about the laminate midplane. This rule applies to both symmetric and antisymmetric angleply stacking sequences. For this reason, cross plies are legitimately represented by the single parameter. The relatively small number of fully orthotropic sequences for thin laminates clearly leaves limited scope for composite tailoring, particularly where ply terminations are necessary and fully orthotropic characteristics are a design requirement. This was the key motivation leading to the redevelopment of the definitive list 3 for specially orthotropic angleply laminates with up to 21 plies, which is presented in a related article in abridged form 4. In the derivation of this list for (but not restricted to) standard angleply configurations, i.e. ±45, 0 and 90, the general rule of symmetry is relaxed. Crossplies, as well as angleplies, are therefore no longer constrained to be symmetric about the laminate midplane, leading to an increase in the number of possible solutions. For 16ply laminates, there are approximately one million possible stacking sequence combinations, of which 368 comply with the requirements of special orthotropy, increasing to approximately 1 billion combinations for 21 plies, giving rise to a hundredfold increase in the number of fully orthotropic laminates. Because of the substantial number of sequences identified in the definitive list, it is beneficial, for design purposes, to express the stiffness properties in terms of lamination parameters, which can be conveniently presented in graphical form, as originally conceived by Fukunaga and Vanderplaats 15 for the purposes of optimum design: the flexural stiffness terms are now fully defined by two linear design variables. Optimized lamination parameters may then be matched against a corresponding set of stacking sequences for a given laminate thickness H (= n t). These graphical representations of feasible domains are readily extended to other laminate classifications: EILs with π/3 ply separation are reduced to a single line representation, whilst π/3 FILs are represented by a single point. II. Stacking sequence derivation In the derivation of the stacking sequences that follow, the general rule of symmetry is relaxed. Cross plies, as well as angle plies, are therefore no longer constrained to be symmetric about the laminate midplane. Consequently, the mixing of 0 and 90 plies needs special attention to avoid violation of the rules for special orthotropy, see Eqs. (3)  (4). There are many nonsymmetric forms contained in the definitive list of fully orthotropic laminates for standard angleply configurations, e.g. ±45, 0 and 90, being both extraordinary in appearance and seemingly infeasible in terms of the uncoupled behavior that the laminates possess. The great majority of sequences are nonsymmetric and many of these are without any subsequence patterns, which is contrary to the assumptions on which many previous studies have been based. Arrangement and form of stacking sequence data For compatibility with the previously published data, similar symbols have been adopted for defining all stacking sequences that follow. Additional symbols and parameters are necessarily included to differentiate between cross plies (0 and 90 ), given that symmetry about the laminate midplane is no longer assumed. The resulting sequences are characterized by subsequence symmetries using a double prefix notation, the first character of which relates to the form of the angleply subsequence and the second character to the crossply subsequence. The double prefix contains combinations of the following characters: A to indicate Antisymmetric form; N for Nonsymmetric; and S for Symmetric. Additionally, for crossply subsequence only, C is used to indicate Crosssymmetric form. To avoid the trivial solution of a stacking sequence with cross plies only, all sequences have an angleply (+) on one outer surface of the laminate. As a result, the other outer surface may have an angleply of equal (+) or opposite ( ) orientation or a cross ply ( ), which may be either 0 or 90. A subscript notation, using these three symbols, is employed to deferential between similar forms of sequence. The form (and number) of FOL stacking sequences contained in the definitive list 3 for up to 21 plies can be summarized as: AC (210), AN (14,532), AS (21,906), SC (12), SN (192), SS (1,029), + NS + (220), + NS (296), + NN + (5,498), + NN (15,188) and + NN = + NN (10,041). From these sequence listings, the form (and number) of the subset for fully uncoupled EIL stacking sequences with π/3 isotropy can be summarized as: AS (173), SS (10), + NN + (106), + NN (208) and + NN = + NN (238), whilst the form (and number) of EIL stacking sequences with π/4 isotropy can be summarized as: AC (12), AS (72), SC (2), SS (6) and + NN = + NN (6). Angleply QHOLs containing a single crossply orientation, i.e. +, and only, can be summarized as: AS (28), SS (4), + NS + (4), + NN + (8), + NN (4) and + NN = + NN (16). 4
5 Development of parameters As adopted in the published ESDU listings 14, the new sequences are ordered in terms of ascending numbers of plies, n, or ζ (= n 3 ), which are in turn ordered by ascending value of the bending stiffness parameter for the angle plies (ζ ± ) and finally by one of the two crossply subsequences (ζ ) within the laminate. Hence, the numbering of sequences for each subsymmetric form, described in the previous section, may be readily extended for higher numbers of plies. All sequences presented in the current article retain their original FOL reference number. The calculation of the bending stiffness parameter, ζ ±, is readily demonstrated for the 9ply fully uncoupled π/3 EIL, designated A382 in the ESDU listings 14 and AS 7 in the definitive list 3, with stacking sequence [±/ / / /+/ /±] T, where the bending stiffness terms, n D ij = Q ij (z k 3 z k1 3 )/3 (8) k = 1 may be written in sequence order for the 9 individual plies, where z, representing the distance from the laminate midplane, is expressed here in terms of the uniform ply thickness t: D ij = {Q ij+ ((7t/2) 3 (9t/2) 3 ) + Q ij ((5t/2) 3 (7t/2) 3 ) + Q ij ( (3t/2) 3 (5t/2) 3 ) + Q ij ((t/2) 3 (3t/2) 3 ) + Q ij ((t/2) 3 (t/2) 3 ) + Q ij+ ((3t/2) 3 (t/2) 3 ) + Q ij ((5t/2) 3 (3t/2) 3 ) + Q ij+ ((7t/2) 3 (5t/2) 3 ) + Q ij ((9t/2) 3 (7t/2) 3 )}/3 (9) where subscripts i, j = 1, 2, 6. The bending stiffness contribution from the angle plies is therefore: and for crossplies: These bending stiffness terms are written in alternative form in Ref. 14 as: and D ij± = 157.5t 3 /3 Q ij± (10) D ij = 24.75t 3 /3 Q ij (11) D ij± = ζ ± t 3 /12 Q ij± (12) D ij = ζ t 3 /12 Q ij (13) respectively, since the number of plies (n = 9) is now related directly to the bending stiffness terms by the expression: ζ ± + ζ = ζ = n 3 (14) where ζ ± = 630 and ζ = n 3 = 729, hence ζ = 99. The stiffness parameters are hereby extended to incorporate both crossplies (ζ and ζ ), including percentage values to indicate the relative proportion (n ± /n, n /n and n /n) and relative contribution to bending stiffness (ζ ± /ζ, ζ /ζ and ζ /ζ) of each ply subsequences within the laminate, i.e. a subsequence containing either ±, or plies. These relationships also help to identify other laminate properties, which are subsets of FOLs. For instance, a QuasiHomogeneous Orthotropic Laminate, or QHOL, has n ± /n = ζ ± /ζ, n /n = ζ /ζ and n /n = ζ /ζ; a π/3 (π/4) 5
6 Extensionally Isotropic Laminate, or EIL, has n ± /n = 2n /n (or = n /n = n /n) and; a π/3 Fully Isotropic Laminate, or FIL, has n ± /n = 2n /n = ζ ± /ζ = 2ζ /ζ. The set of FOLs with up to 21 plies contains no π/4 FILs. Validation The definitive list of FOL stacking sequences, from which the subsets of EILs FILs and QHOLs are derived, have been validated against the published ESDU listing 14, containing symmetric (SS) and antisymmetric (AS) laminates, together with a limited number of nonsymmetric sequences. The laminates detailed in Refs 7, 8, 10 and 16, which have been algorithmically filtered to provide mathematically and mechanically unique stacking sequences, provide further validation. Applying this filtering to the 18 FILs, with π/3 isotropy, identified as a subset of FOLs, which are of the form (and number) + NN + (2), + NN (8) and + NN (8), reveals that: only 1 of the 2 + NN + sequences is unique when the order is reversed, see Fig. 1; only 4 from the 8 + NN sequences are unique when the order is reversed and + and plies are interchanged, see Fig. 2 and; + NN sequences are identical to + NN sequences with and plies interchanged, see Fig. 3, leaving the 5 mathematically and mechanically unique sequences identified by Vannucci and Verchery 8, i.e.: (NN 1071) (NN 1073) (NN 1074) (NN 1075) (NN 1077) [±/ / 3 /+ 2 / /m/±/ 2 / 2 /+] T [+/ / 2 / /+/ /m/±/ /m/ 2 /±] T [+/ / / /m 2 / / / /+/±/ 2 /±] T [+/ 2 / 2 /±/m/+/ 3 /±/ /±] T [+/ / / /m 2 / /m/ 2 /m/+/ / ] T in which +/ / are presented as +60/ 60/0, respectively, in the feasible domains of lamination parameters that follow, but may indeed be any combination of ply angles with π/3 separation; the designations in parentheses correspond to the FOL sequences of Ref. 3. However, the notion of mathematically and mechanically unique stacking sequences is believed to be of limited practical significance, particularly in view of the identical stress distributions of sequences #1 and #4 of Ref. 8, illustrated in Figs 3(g) and 3(e), respectively. This situation arises because the crossply subsequences are identical in these two laminates and, for the particular load combination used, the stress distribution is insensitive to the angleply subsequence. Similarly, laminates NN 1073, 1075, 1081 and 1082, of Figs 2(a), 2(c), 3(c) and 3(a) respectively, have identical stress distributions for the same load combination when the material axis is rotated through 60, i.e. +/ / now represent 0/60/ 60, because the crossply subsequences are identical in all four laminates (a) NN 1071: (b) NN 1071 NN 1072 #5: [±/ / 3 /+ 2 / /m/±/ 2 / 2 /+] T [+/ 2 / 2 /m/±/ /+ 2 / 3 / /m] T Figure 1 Through the thickness stress distribution for fully isotropic, unrestrained laminate (a) NN 1071, and (b) NN 1072 when stacking sequence is reversed, giving rise to sequence #5 of Ref
7 (a) NN 1073: [+/ / 2 / /+/ /m/±/ /m/ 2 /±] T (b) NN 1074: [+/ / / /m 2 / / / /+/±/ 2 /±] T (c) NN 1075: [+/ 2 / 2 /±/m/+/ 3 /±/ /±] T (d) NN 1077: [+/ / / /m 2 / /m/ 2 /m/+/ / ] T (e) NN 1073 NN 1076 [+/ / 2 / /+/ /m/±/ /m/ 2 /±] T (f) NN 1074 NN 1078: [±/ 2 /±/ / /+/ /m 2 / /+/ / ] T (g) NN 1075 NN 1080: [±/ /±/ 3 / 2 /+ 2 /m/+/ 2 / ] T (h) NN 1077 NN 1079 #2: [+/ / /m/ 2 /m/ /m 2 / /+/ / ] T Figure 2 Through the thickness stress distribution for fully isotropic, unrestrained laminates (a) (d) NN 1071 NN 1075 and NN 1077, subject to combined inplane load N x and bending moment M x, and (e) (h) NN 1076, NN 1078 NN 1080 when stacking sequence is reversed and + and plies interchanged; (h) NN 1079 represents sequence #2 of Ref. 8. 7
8 (a) NN 1073 NN 1082: [±/ 2 / /±/ /+ 2 / / / /±/m/ ] T (b) NN 1074 NN 1083: [±/ / / /+/ /±/ /m/+/ / /m/ ] T (c) NN 1075 NN 1081: [±/ / 2 /+/ 2 /+ 2 / 3 /+/ /m/ ] T (d) NN 1077 NN 1084: [±/ / / /+/ /±/ /±/ / /+/±/ ] T (e) NN 1076 NN 1085 #4 [±/ 2 /m/ /±/m/ / / /+ 2 / / ] T (f) NN 1078 NN 1087 #3: [+/ / /m/ 2 /m/ / /+/ /± 2 / ] T (g) NN 1080 NN 1088 #1: [+/ /m/ / 3 / 2 /+ 2 / /+ 2 / 2 / ] T (h) NN 1079 NN 1086: [±/ 2 /±/ / /±/ /+/ /± 2 / ] T Figure 3 Through the thickness stress distribution for fully isotropic, unrestrained laminates (a) (d) NN 1073 NN 1075 and NN 1077, subject to combined inplane load N x and bending moment M x, and (e) (h) NN 1076, NN 1078 NN 1080, resulting from those of Fig. 2 when and plies interchanged, respectively; (g), (f) and (e) giving rise to sequences #1, #3 and #4 of Ref. 8, respectively. Note the identical stress distribution of (e) and (g). 8
9 Figures 1 3 represent the through the thickness stress distributions for unrestrained fully isotropic laminated plates subject to combined inplane load N x (= 4.2 N/mm) and bending moment M x (= 10.0 N.mm/mm). Individual stress distribution profiles arising from the application of N x and M x (dashed lines) are illustrated together with the combined stress distribution profile (solid lines). Material properties and constant ply thickness, t, used in the calculation of these stress distributions, are given in the example calculations that follow. Wu and Avery 5 obtained FILs by varying, or shuffling, the stacking sequences of fully uncoupled EILs in order to produce bending isotropy. Eightynine stacking sequences were presented as the symmetric halves of 36ply laminates with fully isotropic properties, deemed to be the minimum number of plies for π/3 FILs. Limited details of 54ply sequences for FILs with π/3 isotropy are also provided, together with π/4, π/5 and π/6 isotropy for 48, 50 and 72ply sequences, respectively. The symmetry assumption, on which this work is based, precluded the possibility that the listings would contain nonsymmetric 18ply FILs. However, inspection of this list reveals that nine of these stacking sequences represent 18ply nonsymmetric FILs; the nine sequences are reproduced in Table 1 with the original reference numbers and formatting. Table 1 Stacking sequences for 18ply nonsymmetric FILs, representing the symmetric halves of 36ply FILs (after Ref. 5) Ref. θ 1 θ 2 θ Each ply number, 1 through 18, appears under the appropriate plyangle heading, θ 1, θ 2 or θ 3 in row 1 of Table 1. Sequences 57, 65, 66, 70 and 78, correspond to the 5 mechanically and mathematically distinct sequences derived independently by Vannucci and Verchery 8 some ten years later, whilst sequence 69 is sequence 65 with the order reversed and with θ 3, θ 2 and θ 1 in row 1. Similarly, sequences 73, 76 and 77 are, respectively, 66, 57 and 70 with the order reversed and with θ 2, θ 3 and θ 1 in row 1. Sequence AC 127, which is discussed in detail in section V, has special significance: It is a QHOL and validates the unique angleply laminate containing four ply orientations, i.e. +,, and, alluded to in Ref. 16 for a 20 ply laminate satisfying Eq. (7), and Eq. (5) when ply orientations satisfy the π/4 condition, but not Eq. (6). Note that AC 127 and AC 128 are identical when crossplies are interchanged, with. All other QHOLs with up to 21 plies contain either two or three ply orientations, i.e. +, or +, and, respectively. III. Stacking sequence listings The following Tables provide summaries of the numbers of fully uncoupled EIL and QHOL stacking sequences with up to 21 plies together with crossreferences to the Tables of the full sequence listings and nondimensional parameters, given in the appendix. Note that percentage values to indicate the relative proportion (n ± /n, n /n and n /n) and relative contribution to bending stiffness (ζ ± /ζ, ζ /ζ and ζ /ζ) of each ply subsequences within the laminate have been omitted for reasons of compactness, together with other parameters that are common within a given table. These missing parameters are readily calculated from the expressions provided within the table captions. 9
10 Table 2  Number of fully uncoupled π/3 EILs [π/4 EILs] for 7 through 21ply laminates, corresponding to prefix designations for Antisymmetric (A), Crosssymmetric (C), Nonsymmetric (N) and Symmetric (S) ply subsequences, listed in abridged form in Tables 7 and 8. Subscripts arranged before and after the prefix designations denote angle (+, ) and cross plies ( ), and correspond to the orientations of the top and bottom plies of the laminate respectively. Number of plies, n Prefix: Table: AC [2] /[8(a)] AS [2] (a)/[8(b)] SC [2] /[8(c)] +NN (b)/ +NN (c)/ +NN [6] (d)/[8(d)] SS [6] /[8(e)] Table 3  Number of QHOLs containing no crossply orientations for 7 through 21ply laminates, corresponding to prefix designations for Antisymmetric (A), Nonsymmetric (N) and Symmetric (S) ply subsequences, listed in Table 9. Subscripts arranged before and after the prefix designations denote angle (+, ) plies and correspond to the orientations of the top and bottom plies of the laminate respectively. Prefix: Number of plies, n Table: AS (a) +NS (b) +NS 8 9(c) SS 1 9(d) Table 4  Number of QHOLs containing one [both] crossply orientation[s] for 7 through 21ply laminates, corresponding to prefix designations for Antisymmetric (A), Crosssymmetric (C), Nonsymmetric (N) and Symmetric (S) ply subsequences, listed in Table 10. Subscripts arranged before and after the prefix designations denote angle (+, ) and cross plies ( ), and correspond to the orientations of the top and bottom plies of the laminate respectively. Prefix: Number of plies, n Table: AC [2]  AS (a) +NS (b) +NN (c) +NN 4 10(d) +NN (e) SS 4 10(f) 10
11 IV. Calculation of membrane and bending stiffness terms The calculation procedure for the elements (A ij and D ij ) of the extensional (A) and bending (D) stiffness matrices, using the dimensionless parameters provided in Tables 710, are as follows: A ij = {n ± /2 Q ij+ + n ± /2 Q ij + n Q ij + n Q ij } t (15) D ij = {ζ ± /2 Q ij+ + ζ ± /2 Q ij + ζ Q ij + ζ Q ij } t 3 /12 (16) The form of Eqs. (15) and (16) was chosen because they are readily modified to account for laminates with extensional and bending anisotropy by replacing n ± /2 Q ij+ with n ± (n + /n ± )Q ij+ and n ± /2 Q ij with n ± (1 n + /n ± )Q ij, and ζ ± /2 Q ij+ with ζ ± (ζ + /ζ ± ) Q ij+ and ζ ± /2 Q ij with ζ ± (1 ζ + /ζ ± ) Q ij. The use of these modified equation requires the calculation of an additional stiffness parameter, n + and ζ +, relating to the extensional and bending stiffness contribution of positive (θ) angle plies, respectively. The transformed reduced stiffness terms in Eqs. (15) and (16) are given by: and the reduced stiffness terms by: Q 11 = Q 11 cos 4 θ + 2(Q Q 66 )cos 2 θsin 2 θ + Q 22 sin 4 θ Q 12 = Q 21 = (Q 11 + Q 22 4Q 66 )cos 2 θsin 2 θ + Q 12 (cos 4 θ + sin 4 θ) Q 16 = Q 61 = {(Q 11 Q 12 2Q 66 )cos 2 θ + (Q 12 Q Q 66 )sin 2 θ}cosθsinθ Q 22 = Q 11 sin 4 θ + 2(Q Q 66 )cos 2 θsin 2 θ + Q 22 cos 4 θ Q 26 = Q 62 = {(Q 11 Q 12 2Q 66 )sin 2 θ + (Q 12 Q Q 66 )cos 2 θ}cosθsinθ Q 66 = (Q 11 + Q 22 2Q 12 2Q 66 )cos 2 θsin 2 θ + Q 66 (cos 4 θ + sin 4 θ) (17) Q 11 = E 1 /(1 ν 12 ν 21 ) Q 12 = ν 12 E 2 /(1 ν 12 ν 21 ) = ν 21 E 1 /(1 ν 12 ν 21 ) Q 22 = E 2 /(1 ν 12 ν 21 ) Q 66 = G 12 (18) For optimum design of angleply laminates, lamination parameters are often preferred, since these allow the stiffness terms to be expressed as linear variables. The optimized lamination parameters may then be matched against a corresponding set of stacking sequences with given laminate thickness H (= n t). In the context of the parameters presented in the current article, only four of the twelve lamination parameters are required, and these are related through the following expressions: and ξ 1 = ξ 1 A = {n ± (n + /n ± )cos(2θ + ) + n ± (1  n + /n ± )cos(2θ ) + n cos(2θ ) + n cos(2θ )}/n ξ 2 = ξ 2 A = {n ± (n + /n ± )cos(4θ + ) + n ± (1  n + /n ± )cos(4θ ) + n cos(4θ ) + n cos(4θ )}/n (19) ξ 9 = ξ 1 D = {ζ ± (ζ + /ζ ± )cos(2θ + ) + ζ ± (1  ζ + /ζ ± )cos(2θ ) + ζ cos(2θ ) + ζ cos(2θ )}/ζ ξ 10 = ξ 2 D = {ζ ± (ζ + /ζ ± )cos(4θ + ) + ζ ± (1  ζ + /ζ ± )cos(4θ ) + ζ cos(4θ ) + ζ cos(4θ )}/ζ (20) 11
12 where the extensional stiffness parameter n + = (n =) n ± /2 and bending stiffness parameters ζ + (= ζ ) = ζ ± /2 for FOLs, QHOLs, EILs and FILs, hence Eqs. (19) and (20) reduce to: and ξ 1 = {n ± cos(2θ ± ) + n cos(2θ ) + n cos(2θ )}/n ξ 2 = {n ± cos(4θ ± ) + n cos(4θ ) + n cos(4θ )}/n (21) ξ 9 = {ζ ± cos(2θ ± ) + ζ cos(2θ ) + ζ cos(2θ )}/ζ ξ 10 = {ζ ± cos(4θ ± ) + ζ cos(4θ ) + ζ cos(4θ )}/ζ (22) Elements of the extensional and bending stiffness matrices are related to the lamination parameters, respectively, by: and A 11 = {U 1 + ξ 1 U 2 + ξ 2 U 3 } H A 12 = A 21 = {ξ 2 U 3 + U 4 } H A 22 = {U 1 ξ 1 U 2 + ξ 2 U 3 } H A 66 = {ξ 2 U 3 + U 5 } H (23) D 11 = {U 1 + ξ 9 U 2 + ξ 10 U 3 } H 3 /12 D 12 = {U 4 ξ 10 U 3 } H 3 /12 D 22 = {U 1 ξ 9 U 2 + ξ 10 U 3 } H 3 /12 D 66 = {ξ 10 U 3 + U 5 } H 3 /12 (24) where the laminate invariants are given in terms of the reduced stiffnesses of Eq. (18) by: U 1 = {3Q Q Q Q 66 }/8 U 2 = {Q 11 Q 22 }/2 U 3 = {Q 11 + Q 22 2Q 12 4Q 66 }/8 U 4 = {Q 11 + Q Q 12 4Q 66 }/8 U 5 = {Q 11 + Q 22 2Q Q 66 }/8 (25) 12
13 V. Results and Discussion Figure 4(a) (d) illustrates the feasible domains of lamination parameters for all EIL and QHOL subsets from the definitive list of FOLs, in which the +/ / / of Tables 710 correspond to 45/45/0/90, respectively, or 60/ 60/0 for laminates with only one crossply orientation, e.g. π/3 EILs. All membrane (extensional) lamination parameters are bounded by the parabola ξ 2 = 2ξ with limits 1 ξ 1 1and 1 ξ 2 1; for flexural (bending) lamination parameters, ξ 9 and ξ 10 replace ξ 1 and ξ 2, respectively. Stacking sequences lying along the broken line drawn between (ξ 1, ξ 2 ) = (1, 1) and (0, 1) on Fig. 4(a), contain only 0 and ±45 plies, whereas any sequences lying along the line between (0, 1) and (1, 1) would consist of ±45 and 90 plies only. Similarly, any stacking sequences corresponding to the points (1, 1), (0, 1) or (1, 1), would contain only 90 plies, ±45 plies or 0 plies, respectively. A π/3 EIL with 2n ± = n plies, lies at the ⅓ rd point along the line defining a laminate containing only ±60 and 0 plies, i.e. (ξ 1, ξ 2 ) = (0, 0). The flexural lamination parameters corresponding to uncoupled π/3 EILs have orthotropic properties which lie along the line defined by (ξ 9, ξ 10 ) = (1, 1) and (, ) on Fig. 4(b), since the three ply orientations +/ / have been equated to 60/60/0. The flexural lamination parameters corresponding to uncoupled π/4 EILs, illustrated on Fig. 4(c), are contained within the domain defined by the three points corresponding to the 90, ±45 and 0 plies that these sequences contain, cf. Fig. 4(a). All π/3 FILs, with 2ζ ± = ζ, correspond to the point (ξ 1, ξ 2 ) = (ξ 9, ξ 10 ) = (0, 0). QHOLs correspond to any point satisfying (ξ 1, ξ 2 ) = (ξ 9, ξ 10 ) (0, 0). Degenerative QHOLs therefore result from FILs when the π/3 angle separation is relaxed, e.g. where the three ply orientations +/ / correspond to 45/45/0 rather than 60/60/0 : Such sequences are illustrated by the locus of ⅓ rd points shown by the brokenline parabola on Fig. 4(a), representing arbitrary angleply ±θ ±75 ±15 ξ ±60 ±30 ξ ± (a) Domains of membrane lamination parameters for EILs (and FILs with ξ 1 = ξ 2 = 0) and locus (brokenline parabola) for degenerative QHOLs 1.0 ξ 1 (b) Flexural lamination parameters for EILs  π/3 (973) 1.0 ξ 9 ξ ξ2, ξ ξ 9 ξ 1, ξ 9 (c) Flexural lamination parameters for EILs  π/4 (92) (d) Membrane and Flexural lamination parameters for QHOLs (82) with ±θ = 45 ( ) and ±60 ( ) Figure 4 Feasible domains of lamination parameters, in the form of Eqs. (22), for: (a) (c) EILs, including form and number of sequences represented and; (d) the subset of QHOLs from the definitive list of FOLs. 13
14 For IM7/8552 carbonfiber/epoxy material with Young s moduli E 1 = 161.0GPa and E 2 = 11.38GPa, shear modulus G 12 = 5.17GPa and Poison ratio ν 12 = 0.38, lamina thickness t = mm and stacking sequence AC 127: [+/ / 2 / / / / / / /+/ / /+/ /+/ 2 / / ] Τ, the nondimensional parameters are verified by the calculations presented in Table 5, where the first two columns provide the ply number and orientation, respectively. Subsequent columns illustrate the summations, for each ply orientation, of (z k z k1 ), (z k 2 z k1 2 )/2 and (z k 3 z k1 3 )/3, relating to the A, B and D matrices, respectively. The distance from the laminate midplane, z, is expressed in term of ply thickness t, which is set to unit value in the nondimensional expressions. Table 5 Calculation procedure for the nondimensional parameters of the ABD relation. Ply θ (z k z k1 ) A B D AΣ + A Σ A Σ AΣ BΣ + B Σ B Σ BΣ DΣ + D Σ D Σ DΣ 2 (zk z 2 k1 )/2 3 (zk z 3 k1 )/ The nondimensional parameters arising from the summations of Table 5 are: n + (= A Σ + ) = n ± /2 = 4, n = 4, n = 6 and n = 6, and ζ + (= 4 D Σ + ) = 1600, ζ = 1600, ζ = 2400 and ζ = 2400, where n 3 = 20 3 = ζ = ζ + + ζ + ζ + ζ = 8000 and ζ ± = ζ + + ζ = The B matrix summations confirm that B ij = 0 for this laminate. For fiber angles θ = ±45, 0 and 90 in place of symbols ±, and respectively, the transformed reduced stiffnesses are given in Table 6, which are readily calculated using Eqs. (17). 14
15 Table 6 Transformed reduced stiffnesses (N/mm 2 ) for IM7/8552 carbonfiber/epoxy with ply angle θ. θ Q 11 Q 12 Q 16 Q 22 Q 26 Q ,894 40,55437,791 50,89437,791 41, ,894 40,554 37,791 50,894 37,791 41, ,660 4, , , ,497 4, , ,170 and through Eqs. (15) and (16), the final stiffness matrices are derived for the laminate: A11 Sym. A A A A A ,858 52,647 0 = 202,858 0 N/mm Sym. 54,885 D11 Sym. D D D D D ,966 34,249 0 = 131,966 0 N.mm Sym. 35,705 given that: A 16 = {n + Q n Q 16 + n Q 16 + n Q 16 } t A 16 = A 26 = {4 37, , } = 0 N/mm D 16 = {ζ ± /2 Q ζ ± /2 Q 16 + ζ Q 16 + ζ Q 16 } t 3 /12 D 16 = D 26 = { , , } /12 = 0 N.mm This laminate appears to be fully isotropic, since A 11 = A 22 and D ij A ij, but calculation reveals that whilst Eqs. (5) and (7) are satisfied, Eq. (6) is not. Hence this is a Quasi Homogeneous Orthotropic angleply Laminate, or QHOL, containing four ply orientations. The lamination parameters for this laminate, i.e. the coordinates (ξ 1, ξ 2 ) = (ξ 9, ξ 10 ) = (0.0, 0.2) on Fig. 4(d), are derived from Eqs. (21): and Eqs. (22): ξ 1 = {n ± cos(2θ ± ) + n cos(2θ ) + n cos(2θ )}/n ξ 1 = {8 cos(90 ) + 6 cos(0 ) + 6 cos(180 )}/20 = 0.0 ξ 2 = {n ± cos(4θ ± ) + n cos(4θ ) + n cos(4θ )}/n ξ 2 = {8 cos(180 ) + 6 cos(0 ) + 6 cos(360 )}/20 = 0.2 ξ 9 = {ζ ± cos(2θ ± ) + ζ cos(2θ ) + ζ cos(2θ )}/ζ ξ 9 = {3200 cos(90 ) cos(0 ) cos(180 )}/8000 = 0.0 ξ 10 = {ζ ± cos(4θ ± ) + ζ cos(4θ ) + ζ cos(4θ )}/ζ ξ 10 = {3200 cos(180 ) cos(0 ) cos(360 )}/8000 =
16 VI. Conclusions This article presents the definitive set of stacking sequences for (82) QuasiHomogeneous Orthotropic Laminates (QHOLs), (973) π/3 and (92) π/4 Extensionally Isotropic Laminates (EILs) and (36) π/3 Fully Isotropic Laminates (FOLs), all of which are subsets from a definitive list of (69,506) stacking sequences for Fully Orthotropic Laminates (FOLs) with up to 21 plies. The great majority of sequences are nonsymmetric in form and many are without any subsequence patterns, e.g. symmetry or repeating groups, which is contrary to the assumptions on which many previous studies have been based. Standard ply angles (±45 /0 /90 for π/4 isotropy and ±60 /0 for π/3 isotropy) have been assumed in the presentation of the feasible domains of lamination parameters commonly adopted in the optimum design of composite laminates, however the stacking sequences are otherwise generic in the sense that any orientation may be assigned to the angleply subsequence, and the two crossply orientations may be arbitrarily switched. For EIL or FIL properties of course, the choice of these arbitrary ply angles must ensure that π/3 or π/4 ply separation is maintained; the stacking sequences otherwise degenerate into FOLs and QHOLs respectively. The ABD relation has been shown to be readily calculated for any general orthotropic fiber/matrix material using the nondimensional stiffness parameters provided. FILs provide an important set of benchmark configurations, which permit like with like comparisons for laminates with other characteristics. References 1 Engineering Sciences Data Unit, Stiffnesses of laminated plates, ESDU Item No , York, C. B., On composite laminates with extensionalanisotropy, Proc. 49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conf., Schaumburg, Illinois, 2008, Accepted for publication. 3 York, C. B., Laminate stacking sequences for special orthotropy, University of Glasgow, Department of Aerospace Engineering Research Report No , York, C. B., Characterization of nonsymmetric forms of fully orthotropic laminates. AIAA Journal of Aircraft, Accepted for publication. See also, York, C. B. Characterization and ply mixing rules for nonsymmetric forms of fully orthotropic laminates, Proc. 48th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conf., AIAA , Honolulu, Hawaii, Wu, K., M. and Avery, B. L., Fully isotropic laminates and quasihomogeneous anisotropic laminates, Journal of Composite Materials, Vol. 26, No. 14, 1992, pp Fukunaga, H., Sekine, H., Sato, M. and Iino, A., Buckling design of symmetrically laminated plates using lamination parameters Computers and Structures, Vol. 57, No. 4, 1995, pp Valot, E. and Vannucci, P., Some exact solutions for fully orthotropic laminates, Composite Structures, Vol. 69, 2005, pp Vannucci, P. and Verchery, G., A new method for generating fully isotropic laminates, Composite Structures, Vol. 58, 2002, pp Caprino, G. and CrivelliVisconti, I., A note on specially orthotropic laminates, Journal of Composite Materials, Vol. 16, No. 5, 1982, Vannucci, P. and Verchery, G., Stiffness design of laminates using the polar method, International Journal of Solids and Structures, Vol. 38, 2001, pp Tsai, S. W. and Pagano, N. J., Composite materials workshop, in: Tsai S. W. et al., editors, Technomic, USA, Bartholomew, P., Ply stacking sequences for laminated plates having inplane and bending orthotropy, Royal Aircraft Establishment Technical Report No , Bartholomew, P., Ply stacking sequences for laminated plates having inplane and bending orthotropy, Fibre Science and Technology, Vol. 10, No. 4, 1977, pp Engineering Sciences Data Unit, Laminate stacking sequences for special orthotropy (Application to fibre reinforced composites), ESDU Item No , Fukunaga, H., and Vanderplaats, G. N., Stiffness optimization of orthotropic laminated composites using lamination parameters, AIAA Journal, Vol. 29, No. 4, 1991, pp Vannucci, P. and Verchery, G., A special class of uncoupled and quasihomogeneous laminates, Composites Science and Technology, Vol. 61, 2001, pp York, C. B., Buckling interaction in regular arrays of rigidly supported composite laminated plates with orthogrid, isogrid and anisogrid planform, AHS Journal, Vol. 52, No. 4, 2007, pp York, C. B., Buckling analysis and minimum mass design procedures for composite wing box structures, AIAA Journal of Aircraft, Vol. 43, No. 2, 2006, pp
17 Appendix Table 7 Fully uncoupled EILs, with π/3 isotropy, for 7 through 21 ply laminates corresponding to prefix designations: (a) AS for Antisymmetric (A) angleplies and Symmetric (S) crossplies; (b) + NN + for Nonsymmetric (N) angleplies and Nonsymmetric (N) crossplies; (c) + NN and; (d) + NN. For all sequences, n ± = 2n, n = n ± + n and ζ = n 3 = ζ ± + ζ. (a) Ref. Sequence n ζ ± ζ AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS Continued 17
18 Continued AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS Continued 18
19 Continued AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS Continued 19
20 Continued AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS Concluded 20
21 (b) Ref. Sequence n ζ ± ζ NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN Continued 21
A copy can be downloaded for personal noncommercial research or study, without prior permission or charge
York, C. B. (2015) Influence of bending twisting coupling on compression and shear buckling strength. Stability of Structures 14th Symposium, Zakopane, Poland, 812 Jun 2015. Copyright 2015 The Author.
More informationA copy can be downloaded for personal noncommercial research or study, without prior permission or charge
York, C. (2015) On tapered warpfree laminates with singleply terminations. Composites Part A: Applied Science and Manufacturing, 72, pp. 127138. Copyright 2015 Elsevier Ltd. A copy can be downloaded
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationThis is the author s final accepted version.
York, C. B., and Frascino Müller de lmeida, S. (2017) On extensionshearing bendingtwisting coupled laminates. Composite Structures, 164, pp. 1022. (doi:10.1016/j.compstruct.2016.12.041) This is the author
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationLAMINATE DESIGN WITH NONSTANDARD PLY ANGLES FOR OPTIMISED INPLANE PERFORMANCE
21 st International Conference on Composite Materials Xi an, 2025 th August 2017 LAMINATE DESIGN WITH NONSTANDARD PLY ANGLES FOR OPTIMISED INPLANE PERFORMANCE Mark W.D. Nielsen 1, Kevin J. Johnson 1,
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationTHICKNESS TAILORING OF VARIABLE STIFFNESS PANELS FOR MAXIMUM BUCKLING LOAD
THICKNESS TAILORING OF VARIABLE STIFFNESS PANELS FOR MAXIMUM BUCKLING LOAD Samuel T. IJsselmuiden, Mostafa M. Abdalla, Zafer Gürdal Aerospace Structures Chair, Delft University of Technology Kluyverweg
More informationSTRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES
ECCM1616 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 214 STRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES M. Nielsen a, A. T. Rhead a,
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationON THE NUMERICAL ANALYSIS OF COMPOSITE MATERIAL
The 4th International Conference Advanced Composite Materials Engineering COMAT 8 October, Brasov, Romania O THE UMERICAL AALYSIS OF COMPOSITE MATERIAL D.D. icoara Transilvania University, City Brasov,
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationVIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS
VIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS Mechanical Engineering Department, Indian Institute of Technology, New Delhi 110 016, India (Received 22 January 1992,
More informationThe Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries
The Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries M. D. Thouless Department of Mechanical Engineering Department of Materials Science & Engineering University
More informationImproved Design Formulae for Buckling of Orthotropic Plates under Combined Loading
Improved Design Formulae for Buckling of Orthotropic Plates under Combined Loading Paul M. Weaver 1 University of Bristol, Bristol, England BS8 1TR, United Kingdom Michael P. Nemeth 2 NASA Langley Research
More informationA short review of continuum mechanics
A short review of continuum mechanics Professor Anette M. Karlsson, Department of Mechanical ngineering, UD September, 006 This is a short and arbitrary review of continuum mechanics. Most of this material
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationTHE NETTING ANALYSIS AS A LIMIT CASE OF THE LAMINATED STRUCTURE THEORY
THE NETTING ANALYSIS AS A LIMIT CASE OF THE LAMINATED STRUCTURE THEORY G. Verchery Pluralis, SaintÉtienne, France Georges.Verchery@m4x.org Keywords: netting analysis, classical laminated plate theory,
More information46th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference April 2005 Austin, Texas
th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference  April, Austin, Texas AIAA  AIAA  Bistable Cylindrical Space Frames H Ye and S Pellegrino University of Cambridge, Cambridge,
More informationLinear elastic analysis of thin laminated beams with uniform and symmetric crosssection
Applied and Computational Mechanics 2 (2008) 397 408 Linear elastic analysis of thin laminated beams with uniform and symmetric crosssection M. Zajíček a, a Faculty of Applied Sciences, UWB in Pilsen,
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationXI. NANOMECHANICS OF GRAPHENE
XI. NANOMECHANICS OF GRAPHENE Carbon is an element of extraordinary properties. The carboncarbon bond possesses large magnitude cohesive strength through its covalent bonds. Elemental carbon appears in
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 34 Thermal Stresses in Plates Lecture Overview Introduction Mechanical and Thermal Strains
More informationFLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR DEFORMABLE PLATE THEORY
AsiaPacific Conference on FRP in Structures (APFIS 2007) S.T. Smith (ed) 2007 International Institute for FRP in Construction FLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR
More informationLearning Units of Module 3
Module Learning Units of Module M. tresstrain oncepts in Three Dimension M. Introduction to Anisotropic lasticity M. Tensorial oncept and Indicial Notations M.4 Plane tress oncept Action of force (F)
More informationComposite Structural Mechanics using MATLAB
Session 2520 Composite Structural Mechanics using MATLAB Oscar Barton, Jr., Jacob B. Wallace United States Naval Academy Annapolis, Md 21402 Abstract In this paper MATLAB is adopted as the programming
More informationThe stiffness of plates
The stiffness of plates 1. Introduction The word plate is a collective term for elements in which forces can be transferred in two directions. Floors, walls, bridge slabs and laminates are all plates.
More informationOnline publication date: 23 October 2010
This article was downloaded by: [informa internal users] On: 1 November 2010 Access details: Access Details: [subscription number 755239602] Publisher Taylor & Francis Informa Ltd Registered in England
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationKeywords: Adhesively bonded joint, laminates, CFRP, stacking sequence
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS GLOBAL AND LOCAL INFLUENCE OF STACKING SEQUENCE ON THE STRENGTH OF ADHESIVELY BONDED JOINTS OF CFRP LAMINATES J. Rousseau*, P. Satthamnuwong DRIVE,
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationFOLDING AND DEPLOYMENT OF ULTRATHIN COMPOSITE STRUCTURES
FOLDING AND DEPLOYMENT OF ULTRATHIN COMPOSITE STRUCTURES H.M.Y.C. Mallikarachchi (1), S. Pellegrino (2) (1) University of Cambridge Department of Engineering, Trumpington Street, Cambridge CB2 1PZ, U.K.
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More informationCOMPARISON OF PLATE MODELS FOR ANALYSIS OF LAMINATED COMPOSITES
COMPARISON OF PLATE MODELS FOR ANALYSIS OF LAMINATED COMPOSITES P. M. Mohite and C. S. Upadhyay** Department of Aerospace Engineering, IIT Kanpur 0806, INDIA, email: mohite@iitk.ac.in Assistant Professor,
More informationAPPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS
APPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS L. Zu, S. Koussios and A. Beukers Design and Production of Composite Structures, Faculty of Aerospace Engineering
More informationVIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS
Journal of Engineering Science and Technology Vol. 12, No. 12 (217) 33983411 School of Engineering, Taylor s University VIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS DILEEP
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationFree Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires
11(2014) 279298 Free Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires Abstract In this paper, free vibration response of a hybrid composite plate was studied. Effects
More informationGetting Started with Composites Modeling and Analysis
Getting Started with Composites Modeling and Analysis IN THIS WEBINAR: PRESENTED BY: Orthotropic materials and how to define them Composite Laminate properties and modeling Composite failure theories and
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationAs an example we consider the stacking and analysis of a 2ply symmetric laminate. First we clear the Matlab space and close figures.
Program Lam 1 Introduction The collection of Matlab command and function files in the package lam allows the stacking and analysis of a laminate. In fact only a representative piece of a laminate is considered,
More informationThermal buckling and postbuckling of laminated composite plates with. temperature dependent properties by an asymptotic numerical method
hermal buckling and postbuckling of laminated composite plates with temperature dependent properties by an asymptotic numerical method F. Abdoun a,*, L. Azrar a,b, E.M. Daya c a LAMA, Higher School of
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationAnalysis of NonRectangular Laminated Anisotropic Plates by Chebyshev Collocation Method
146 Analysis of NonRectangular Laminated Anisotropic Plates by Chebyshev Collocation Method ChihHsun LIN and MingHwa R. JEN The purpose of this work is to solve the governing differential equations
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationCombined Stresses and Mohr s Circle. General Case of Combined Stresses. General Case of Combined Stresses con t. Twodimensional stress condition
Combined Stresses and Mohr s Circle Material in this lecture was taken from chapter 4 of General Case of Combined Stresses Twodimensional stress condition General Case of Combined Stresses con t The normal
More informationFinite Element and Plate Theory Modeling of Acoustic Emission Waveforms. NASA Langley Research Center. Hampton, VA *University of Denver
Finite Element and Plate Theory Modeling of Acoustic Emission Waveforms W. H. Prosser, M. A. Hamstad + *, J. Gary +, and A. O Gallagher + NASA Langley Research Center Hampton, VA 236811 *University of
More informationChapter 5 PlaneStress StressStrain Relations in a Global Coordinate System
Chapter 5 PlaneStress StressStrain Relations in a Global Coordinate System One of the most important characteristics of structures made of fiberreinforced materials, and one which dictates the manner
More informationShishir Kumar Sahu, Ph. D. Professor Civil Engineering Department National Institute of Technology, Rourkela Orissa, India
Shishir Kumar Sahu, Ph. D. Professor Civil Engineering Department National Institute of Technology, Rourkela Orissa, India Introduction Review Of Literature Aim & Scope Of Present Investigation Finite
More informationCOMPOSITE PLATE THEORIES
CHAPTER2 COMPOSITE PLATE THEORIES 2.1 GENERAL Analysis of composite plates is usually done based on one of the following the ries. 1. Equivalent singlelayer theories a. Classical laminate theory b. Shear
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationDesign and optimization of a variable stiffness composite laminate
th World Congress on Structural and Multidisciplinary Optimisation 07 th  th, June 05, Sydney Australia Design and optimization of a variable stiffness composite laminate Yan Zhang, Fenfen Xiong Qian
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationMATERIAL PROPERTIES. Material Properties Must Be Evaluated By Laboratory or Field Tests 1.1 INTRODUCTION 1.2 ANISOTROPIC MATERIALS
. MARIAL PROPRIS Material Properties Must Be valuated By Laboratory or Field ests. INRODUCION he fundamental equations of structural mechanics can be placed in three categories[]. First, the stressstrain
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationBuckling Behavior of Long Symmetrically Laminated Plates Subjected to Shear and Linearly Varying Axial Edge Loads
NASA Technical Paper 3659 Buckling Behavior of Long Symmetrically Laminated Plates Sujected to Shear and Linearly Varying Axial Edge Loads Michael P. Nemeth Langley Research Center Hampton, Virginia National
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationConstitutive model for quasistatic deformation of metallic sandwich cores
INTERNATIONAL JOURNAL FOR NUMERICAL METHODS IN ENGINEERING Int. J. Numer. Meth. Engng 2004; 61:2205 2238 Published online 18 October 2004 in Wiley InterScience (www.interscience.wiley.com). DOI: 10.1002/nme.1142
More informationDesign of Pressure Vessel Pads and Attachments To Minimize Global Stress Concentrations
Transactions, SMiRT 9, Toronto, August 007 Design of Pressure Vessel Pads and Attachments To Minimize Global Stress Concentrations Gordon S. Bjorkman ) ) Spent Fuel Storage and Transportation Division,
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationApplication of piezoelectric actuators to active control of composite spherical caps
Smart Mater. Struct. 8 (1999 18. Printed in the UK PII: S964176(9916614 Application of piezoelectric actuators to active control of composite spherical caps Victor Birman, Gareth J Knowles and John J
More informationUsing the finite element method of structural analysis, determine displacements at nodes 1 and 2.
Question 1 A pinjointed plane frame, shown in Figure Q1, is fixed to rigid supports at nodes and 4 to prevent their nodal displacements. The frame is loaded at nodes 1 and by a horizontal and a vertical
More informationThe Rotating Inhomogeneous Elastic Cylinders of. VariableThickness and Density
Applied Mathematics & Information Sciences 23 2008, 237 257 An International Journal c 2008 Dixie W Publishing Corporation, U. S. A. The Rotating Inhomogeneous Elastic Cylinders of VariableThickness and
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationApplication of Laplace Iteration method to Study of Nonlinear Vibration of laminated composite plates
(3) 78 795 Application of Laplace Iteration method to Study of Nonlinear Vibration of laminated composite plates Abstract In this paper, free vibration characteristics of laminated composite plates are
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationBISTABLE COMPOSITE SHELLS
AIAA 21385 BISTABLE COMPOSITE SHELLS K. Iqbal and S. Pellegrino Department of Engineering, University of Cambridge, Trumpington Street, Cambridge, CB2 1PZ, U.K. Abstract This paper is concerned with
More informationComposite angle ply laminates and netting analysis
10.1098/rspa.2002.1066 FirstCite epublishing Composite angle ply laminates and netting analysis By J. T. Evans and A. G. Gibson School of Mechanical and Systems Engineering, University of Newcastle upon
More informationA STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS
Xi an, 225 th August 217 A STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS LI Zhongyang 1, LI Dong 2 Mailbox7235, Yanliang District, Xian, China, Email: zhongyangli@live.com Keywords:
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationCSMA Introduction. M. Brunetti 1, A. Vincenti 2, S. Vidoli 3
CS017 13ème Colloque National en Calcul des Structures 1519 Mai 017, Presqu île de Giens (Var) 13ème Colloque National en Calcul des Structures Multistable shell structures satisfying clamped boundary
More informationClassical Lamination Theory: The Kirchhoff Hypothesis
212 Chapter 6 Classical Lamination Theory: The Kirchhoff Hypothesis In the preceding chapters we developed the tools needed to understand the elastic response of a small volume of fiberreinforced material
More information